| ||Format||Pages||Price|| |
|10||$48.00||  ADD TO CART|
|Hardcopy (shipping and handling)||10||$48.00||  ADD TO CART|
Significance and Use
5.1 The strength and performance of heat-strengthened and fully-tempered glass is greatly affected by the surface and edge stress induced during the heat-treating process.
5.2 The edge and surface stress levels are specified in Specification , in the Engineering Standards Manual of GANA Tempering Division and in foreign specifications.
5.3 This test method offers a direct and convenient way to non-destructively determine the residual state of stress on the surface and at the edge of annealed and heat-treated glass.
1.1 This test method covers the determination of edge stresses and surface stresses in annealed, heat-strengthened, and fully tempered flat glass products.
1.2 This test method is non-destructive.
1.3 This test method uses transmitted light and is, therefore, applicable to light-transmitting glasses.
1.4 The test method is not applicable to chemically-tempered glass.
1.5 Using the procedure described, surface stresses can be measured only on the “tin” side of float glass.
1.6 Surface-stress measuring instruments are designed for a specific range of surface index of refraction.
1.7 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.8 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.9 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C158 Test Methods for Strength of Glass by Flexure (Determination of Modulus of Rupture)
C162 Terminology of Glass and Glass Products
C770 Test Method for Measurement of Glass StressOptical Coefficient
C1048 Specification for Heat-Strengthened and Fully Tempered Flat Glass
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
Other Documents“Surface and Edge Stress in Tempered Glass Engineering Standards Manual Available from Glass
ICS Number Code 81.040.20 (Glass in building)
UNSPSC Code 30171706(Tempered glass)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM C1279-13(2019), Standard Test Method for Non-Destructive Photoelastic Measurement of Edge and Surface Stresses in Annealed, Heat-Strengthened, and Fully Tempered Flat Glass, ASTM International, West Conshohocken, PA, 2019, www.astm.orgBack to Top